# Entangled polymer beaucag/Classes/Properties/Physics... Entangled polymer dynamics 9.1 Entanglements

• View
0

0

Embed Size (px)

### Text of Entangled polymer beaucag/Classes/Properties/Physics... Entangled polymer dynamics 9.1 Entanglements

• Entangled polymer dynamics

9.1 Entanglements in polymer melts

The Edwards tube model of polymer entanglements was already discussed in Section 7.3.1. The topological constraints imposed by neighbouring chains on a given chain restrict its motion to a tube-like region (see Fig. 7.10) called the confining tube. The motion of the chain along the contour of the tube (the primitive path) is unhindered by topological interactions. Displacement of monomers in the direction perpendicular to the primitive path is restricted by surrounding chains to an average distance u, called the tube diameter. The number of Kuhn monomers in a strand of size equal to the amplitude of transverse fluctuations (the tube diameter) is N,, the number of monomers in an entanglement strand. For melts, excluded volume interactions are screened (see Section 4.5.2) and the tube diameter is determined by ideal chain statistics:

u E h a . (9.1)

The tube can be thought of as being composed of N I N , sections of size u, with each section containing N , monomers. The chain can be considered as either a random walk of entanglement strands ( N I N , strands of size u) or a random walk of monomers ( N monomers of size b).

The average contour length (L) of the primitive path (the centre of the confining tube, see Fig. 7.10) is the product of the entanglement strand length u and the average number of entanglement strands per chain NIN,.

The average primitive path contour length (L) is shorter than the contour length of the chain hN by the factor u lh E because each entanglement strand in a melt is a random walk of N, Kuhn monomers.

One manifestation of entanglement in long chains (N>>N,) is the appearance of a wide region in time (or frequency) where the modulus is

• 3 62 Entangled polymer dynamics

almost constant in a stress relaxation (or oscillatory shear) experiment. In analogy with crosslinked rubbers, this region is referred to as the rubbery plateau, and the nearly constant value of the modulus in this plateau regime is called the plateau modulus G,. In analogy with an affine network, whose modulus is of order kT per network strand [Eq. (7.31)], the plateau modulus is of order kT per entanglement strand [Eq.(7.47)]. The number- average molar mass of an entanglement strand is called the entanglement molar mass Me. The occupied volume of an entanglement strand with molar mass Me in a melt with density p is the product of the number of Kuhn monomers per strand N, and the Kuhn monomer volume vo:

Since monomers are space-filling in the melt, the number density of entanglement strands is just the reciprocal of the entanglement strand volume, leading to a simple expression for the plateau modulus of an entangled polymer melt [Eq. (7.47)].

Ge=---- pRT kT h 'kT N N--.

Me voNe voa2h (9.5)

The number of chains P, within the confinement volume u3 is deter- mined from the fact that monomers in the melt are space-filling:

Table 9.1 shows N, and P, calculated from the measured plateau modulus. All flexible polymers have P, cz 20 overlapping entanglement strands defining the entanglement volume u3, which is the overlap criterion for entanglement in polymer melts.

Table 9.1 Entanglement parameters for flexible linear polymer melts

Polyethylene at 140 " C Poly(ethy1ene oxide)

1,4-PoIybutadiene at 25 "C Polypropylene at 140 "C 1,4-Polyisoprene at 25 "C Polyiaobutylene at 25 "C Polydimethylsiloxane

Polystyrene at 140 " C Pol yvin ylcyclohexane

dt 80°C

dt 25 "c

at 160°C

2.6 1.8

1.15 0.47 0.35 0.34 0.20

0.20 0.068

1000 1700

1900 5800 6400 6700

12 000

17 000 49 000

7 14 36 320 21 13 11 37 210 19

18 10 41 190 19 32 11 62 380 20 53 8.4 62 220 20 24 13 62 500 19 32 13 74 650 20

23 18 85 1200 22 81 14 130 1100 22

• Reptation in polymer melts

9.2 Reptation in polymer melts

363

At first glance, understanding the motion of a polymer in the melt is daunting. Since roughly fi other polymers share the pervaded volume of a given chain in the melt, chain motion appears to be a difficult many- body problem. However, by utilizing the Edwards tube concept, de Gennes cleverly reduced this many-body problem to the motion of a single chain confined to a tube of surrounding chains. Models that con- sider chain motion as being restricted to a tube-like region are referred to as tube models. The simplest tube model was proposed by de Gennes in 197 1 for the motion of linear entangled polymers, and is called the reptation model.

9.2.1 Relaxation times and diffusion

In de Gennes' reptation model, an entangled chain diffuses along its confining tube in a way analogous to the motion of a snake or a worm (see Fig. 9.1). This motion of the chain consists of diffusion of small loops, along the contour of the primitive path. This curvilinear motion of a polymer along its tube satisfies the topological constraints imposed by surrounding chains and is characterized by the Rouse friction coefficient NC. The curvilinear diffusion coefficient D, that describes motion of the chain along its tube is simply the Rouse diffusion coefficient of the chain [Eq. (8.12)].

kT NC D p-. (9.7)

The time it takes for the chain to diffuse out of the original tube of average length (L) is the reptation time:

Fig. 9.1 Reptation steps: (a) formation of a loop at the tail of the snake and elimination of the tail segment of the confining tube; (b) propagation of the loop along the contour of the tube; (c) release of the loop at the head ofthe snake and formatioll of a new sectioll of the confining tube.

%---- (9.8)

Here, Eq. (9.3) was used for the average contour length of the tube. The reptation time rrep is predicted to be proportional to the cube of the molar mass. The experimentally measured scaling exponent is higher than 3:

r N M3.4. (9.9)

We will discuss the possible reasons for the disagreement between the simple reptation model and experiments in Section 9.4.5.

The first part of the final relation of Eq. (9.8) is the Rouse time of an entanglement strand containing N , monomers:

(9.10)

• 3 64 Entangled polymer dynamics

The ratio of the reptation time rreP and re is the cube of the number of entanglements along the chain:

1 O-lo I

M (g mol-')

Fig. 9.2 Molar mass dependence of the diffusion coefficient for melts of hydrogenated polybutadieiie at 175 "C. Data compiled in T. P. Lodge Phys. Rev. Lett. 83, 3218 (1999).

(9.1 1)

The chain moves a distance of order of its own size R in its reptation time rrep, since this is the time scale at which the tube is abandoned:

R2 k T N , Drep z ~ ~z -- rrep C N 2 ' (9.12)

The diffusion coefficient of entangled linear polymers is predicted to be reciprocally proportional to the square of the molar mass, which also disagrees with experiments, as shown in Fig. (9.2):

D % - w R2 M-2.3 r

(9.13)

9.2.2 Stress relaxation and viscosity

The reptation ideas discussed above will now be combined with the relaxation ideas discussed in Chapter 8 to describe the stress relaxation modulus G(t) for an entangled polymer melt. On length scales smaller than the tube diameter a, topological interactions are unimportant and the dynamics are similar to those in unentangled polymer melts and are described by the Rouse model. The entanglement strand of Ne monomers relaxes by Rouse motion with relaxation time re [Eq. (9.10)]:

re = TON:. (9.14)

The Rouse model predicts that the stress relaxation modulus on these short time scales decays inversely proportional to the square root of time [Eq. (8.47)]:

-112

for TO < t < re. (9.15)

The relaxation time of the Kuhn monomer ro is the shortest stress relaxation time in the Rouse model, given by Eq. (8.56) with p = N:

Cb2 Cb2 67r2kT kT

To=-%-. (9.16)

The stress relaxation modulus at ro is the Kuhn modulus (kT per Kuhn monomer):

(9.17)

• Reptation in polymer melts 365

I"

10-210-1 1 10' lo2 lo3 lo4 lo5 lo6 lo7 l ox amT (radk)

Consider for example, a melt of 1,4-polybutadiene linear chains with M = 130000gmolp'. The molar mass of a polybutadiene Kuhn monomer is Mo= 105gmolp' (see Table 2.1) so this chain has N = M/Mo = 1240 Kuhn monomers. At 25 "C, this polymer is 124 K above its glass transition and its oscillatory shear master curve is shown in Fig. 9.3. The time scale for monomer motion is ro cz 0.3 ns, An entanglement strand of 1,4-polybutadiene has molar mass M, = 1900 gmolp' (see Table 9.1) and therefore contains N , = M,/Mo = 18 Kuhn monomers. The whole chain has N/N,=M/M,=68 entanglements. The Rouse time of the entanglement strand re E 0.1 ps [Eq. (9. lo)].

At the Rouse time of an entanglement strand re, the chain 'finds out' that its motion is topologically hindered by surrounding chains. Free Rouse motion of the chain is no longer possible on time scales t > T,. The value of the stress relaxation modulus at r, is the plateau modulus G,, which is kT per entanglement strand [Eq. (9.5)]:

The Rouse time of the chain is rR cz 0.5 ms:

(9.18)

(9.19)

In the simple reptation model, there is a delay in relaxation (the rubbery plateau) between re and the reptation time of the chain rrep [Eq. (9.1 l)]. By restricting the chain's Rouse motions to t

Recommended

Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents
Documents